LMucko/crystallography-open-database huggingface dataset:
Thermal expansion of periclase (MgO) and tungsten (W) to melting temperatures Sample: T = 455 K
Dubrovinsky, L. S.; Saxena, S. K.; Physics and Chemistry of Minerals 24 (1997) 547–550; doi:10.1007/s002690050070

data_9006487
_publ_section_title
;
 Thermal expansion of periclase (MgO) and tungsten (W)
 to melting temperatures
 Sample: T = 455 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              547
_journal_page_last               550
_journal_paper_doi               10.1007/s002690050070
_journal_volume                  24
_journal_year                    1997
_chemical_formula_sum            W
_chemical_name_mineral           Tungsten
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.1672
_cell_length_b                   3.1672
_cell_length_c                   3.1672
_cell_formula_units_Z            2
_cell_volume                     31.771
_database_code_amcsd             0008069
_diffrn_ambient_temperature      455
_exptl_crystal_density_diffrn    19.218
_cod_original_sg_symbol_H-M      'I m 3 m'
_cod_database_code               9006487
Thermal expansion of periclase (MgO) and tungsten (W) to melting temperatures Sample: T = 905 K
Dubrovinsky, L. S.; Saxena, S. K.; Physics and Chemistry of Minerals 24 (1997) 547–550; doi:10.1007/s002690050070

data_9006488
_publ_section_title
;
 Thermal expansion of periclase (MgO) and tungsten (W)
 to melting temperatures
 Sample: T = 905 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              547
_journal_page_last               550
_journal_paper_doi               10.1007/s002690050070
_journal_volume                  24
_journal_year                    1997
_chemical_formula_sum            W
_chemical_name_mineral           Tungsten
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.1731
_cell_length_b                   3.1731
_cell_length_c                   3.1731
_cell_formula_units_Z            2
_cell_volume                     31.949
_database_code_amcsd             0008070
_diffrn_ambient_temperature      905
_exptl_crystal_density_diffrn    19.111
_cod_original_sg_symbol_H-M      'I m 3 m'
_cod_database_code               9006488
Thermal expansion of periclase (MgO) and tungsten (W) to melting temperatures Sample: T = 918 K
Dubrovinsky, L. S.; Saxena, S. K.; Physics and Chemistry of Minerals 24 (1997) 547–550; doi:10.1007/s002690050070

data_9006489
_publ_section_title
;
 Thermal expansion of periclase (MgO) and tungsten (W)
 to melting temperatures
 Sample: T = 918 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              547
_journal_page_last               550
_journal_paper_doi               10.1007/s002690050070
_journal_volume                  24
_journal_year                    1997
_chemical_formula_sum            W
_chemical_name_mineral           Tungsten
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.1738
_cell_length_b                   3.1738
_cell_length_c                   3.1738
_cell_formula_units_Z            2
_cell_volume                     31.970
_database_code_amcsd             0008071
_diffrn_ambient_temperature      918
_exptl_crystal_density_diffrn    19.099
_cod_original_sg_symbol_H-M      'I m 3 m'
_cod_database_code               9006489
Thermal expansion of periclase (MgO) and tungsten (W) to melting temperatures Sample: T = 1205 K
Dubrovinsky, L. S.; Saxena, S. K.; Physics and Chemistry of Minerals 24 (1997) 547–550; doi:10.1007/s002690050070

data_9006490
_publ_section_title
;
 Thermal expansion of periclase (MgO) and tungsten (W)
 to melting temperatures
 Sample: T = 1205 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              547
_journal_page_last               550
_journal_paper_doi               10.1007/s002690050070
_journal_volume                  24
_journal_year                    1997
_chemical_formula_sum            W
_chemical_name_mineral           Tungsten
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.1775
_cell_length_b                   3.1775
_cell_length_c                   3.1775
_cell_formula_units_Z            2
_cell_volume                     32.082
_database_code_amcsd             0008072
_diffrn_ambient_temperature      1205
_exptl_crystal_density_diffrn    19.032
_cod_original_sg_symbol_H-M      'I m 3 m'
_cod_database_code               9006490
Thermal expansion of periclase (MgO) and tungsten (W) to melting temperatures Sample: T = 1363 K
Dubrovinsky, L. S.; Saxena, S. K.; Physics and Chemistry of Minerals 24 (1997) 547–550; doi:10.1007/s002690050070

data_9006491
_publ_section_title
;
 Thermal expansion of periclase (MgO) and tungsten (W)
 to melting temperatures
 Sample: T = 1363 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              547
_journal_page_last               550
_journal_paper_doi               10.1007/s002690050070
_journal_volume                  24
_journal_year                    1997
_chemical_formula_sum            W
_chemical_name_mineral           Tungsten
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.1804
_cell_length_b                   3.1804
_cell_length_c                   3.1804
_cell_formula_units_Z            2
_cell_volume                     32.170
_database_code_amcsd             0008073
_diffrn_ambient_temperature      1363
_exptl_crystal_density_diffrn    18.980
_cod_original_sg_symbol_H-M      'I m 3 m'
_cod_database_code               9006491
Thermal expansion of periclase (MgO) and tungsten (W) to melting temperatures Sample: T = 1410 K
Dubrovinsky, L. S.; Saxena, S. K.; Physics and Chemistry of Minerals 24 (1997) 547–550; doi:10.1007/s002690050070

data_9006492
_publ_section_title
;
 Thermal expansion of periclase (MgO) and tungsten (W)
 to melting temperatures
 Sample: T = 1410 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              547
_journal_page_last               550
_journal_paper_doi               10.1007/s002690050070
_journal_volume                  24
_journal_year                    1997
_chemical_formula_sum            W
_chemical_name_mineral           Tungsten
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.1822
_cell_length_b                   3.1822
_cell_length_c                   3.1822
_cell_formula_units_Z            2
_cell_volume                     32.224
_database_code_amcsd             0008074
_diffrn_ambient_temperature      1410
_exptl_crystal_density_diffrn    18.948
_cod_original_sg_symbol_H-M      'I m 3 m'
_cod_database_code               9006492
Thermal expansion of periclase (MgO) and tungsten (W) to melting temperatures Sample: T = 1527 K
Dubrovinsky, L. S.; Saxena, S. K.; Physics and Chemistry of Minerals 24 (1997) 547–550; doi:10.1007/s002690050070

data_9006493
_publ_section_title
;
 Thermal expansion of periclase (MgO) and tungsten (W)
 to melting temperatures
 Sample: T = 1527 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              547
_journal_page_last               550
_journal_paper_doi               10.1007/s002690050070
_journal_volume                  24
_journal_year                    1997
_chemical_formula_sum            W
_chemical_name_mineral           Tungsten
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.1837
_cell_length_b                   3.1837
_cell_length_c                   3.1837
_cell_formula_units_Z            2
_cell_volume                     32.270
_database_code_amcsd             0008075
_diffrn_ambient_temperature      1527
_exptl_crystal_density_diffrn    18.921
_cod_original_sg_symbol_H-M      'I m 3 m'
_cod_database_code               9006493
Thermal expansion of periclase (MgO) and tungsten (W) to melting temperatures Sample: T = 1537 K
Dubrovinsky, L. S.; Saxena, S. K.; Physics and Chemistry of Minerals 24 (1997) 547–550; doi:10.1007/s002690050070

data_9006494
_publ_section_title
;
 Thermal expansion of periclase (MgO) and tungsten (W)
 to melting temperatures
 Sample: T = 1537 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              547
_journal_page_last               550
_journal_paper_doi               10.1007/s002690050070
_journal_volume                  24
_journal_year                    1997
_chemical_formula_sum            W
_chemical_name_mineral           Tungsten
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.1824
_cell_length_b                   3.1824
_cell_length_c                   3.1824
_cell_formula_units_Z            2
_cell_volume                     32.230
_database_code_amcsd             0008076
_diffrn_ambient_temperature      1537
_exptl_crystal_density_diffrn    18.944
_cod_original_sg_symbol_H-M      'I m 3 m'
_cod_database_code               9006494
Thermal expansion of periclase (MgO) and tungsten (W) to melting temperatures Sample: T = 1685 K
Dubrovinsky, L. S.; Saxena, S. K.; Physics and Chemistry of Minerals 24 (1997) 547–550; doi:10.1007/s002690050070

data_9006495
_publ_section_title
;
 Thermal expansion of periclase (MgO) and tungsten (W)
 to melting temperatures
 Sample: T = 1685 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              547
_journal_page_last               550
_journal_paper_doi               10.1007/s002690050070
_journal_volume                  24
_journal_year                    1997
_chemical_formula_sum            W
_chemical_name_mineral           Tungsten
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.1866
_cell_length_b                   3.1866
_cell_length_c                   3.1866
_cell_formula_units_Z            2
_cell_volume                     32.358
_database_code_amcsd             0008077
_diffrn_ambient_temperature      1685
_exptl_crystal_density_diffrn    18.869
_cod_original_sg_symbol_H-M      'I m 3 m'
_cod_database_code               9006495
Thermal expansion of periclase (MgO) and tungsten (W) to melting temperatures Sample: T = 1846 K
Dubrovinsky, L. S.; Saxena, S. K.; Physics and Chemistry of Minerals 24 (1997) 547–550; doi:10.1007/s002690050070

data_9006496
_publ_section_title
;
 Thermal expansion of periclase (MgO) and tungsten (W)
 to melting temperatures
 Sample: T = 1846 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              547
_journal_page_last               550
_journal_paper_doi               10.1007/s002690050070
_journal_volume                  24
_journal_year                    1997
_chemical_formula_sum            W
_chemical_name_mineral           Tungsten
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.1913
_cell_length_b                   3.1913
_cell_length_c                   3.1913
_cell_formula_units_Z            2
_cell_volume                     32.501
_database_code_amcsd             0008078
_diffrn_ambient_temperature      1846
_exptl_crystal_density_diffrn    18.786
_cod_original_sg_symbol_H-M      'I m 3 m'
_cod_database_code               9006496
Thermal expansion of periclase (MgO) and tungsten (W) to melting temperatures Sample: T = 1870 K
Dubrovinsky, L. S.; Saxena, S. K.; Physics and Chemistry of Minerals 24 (1997) 547–550; doi:10.1007/s002690050070

data_9006497
_publ_section_title
;
 Thermal expansion of periclase (MgO) and tungsten (W)
 to melting temperatures
 Sample: T = 1870 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              547
_journal_page_last               550
_journal_paper_doi               10.1007/s002690050070
_journal_volume                  24
_journal_year                    1997
_chemical_formula_sum            W
_chemical_name_mineral           Tungsten
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.1908
_cell_length_b                   3.1908
_cell_length_c                   3.1908
_cell_formula_units_Z            2
_cell_volume                     32.486
_database_code_amcsd             0008079
_diffrn_ambient_temperature      1870
_exptl_crystal_density_diffrn    18.795
_cod_original_sg_symbol_H-M      'I m 3 m'
_cod_database_code               9006497
Thermal expansion of periclase (MgO) and tungsten (W) to melting temperatures Sample: T = 2032 K
Dubrovinsky, L. S.; Saxena, S. K.; Physics and Chemistry of Minerals 24 (1997) 547–550; doi:10.1007/s002690050070

data_9006498
_publ_section_title
;
 Thermal expansion of periclase (MgO) and tungsten (W)
 to melting temperatures
 Sample: T = 2032 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              547
_journal_page_last               550
_journal_paper_doi               10.1007/s002690050070
_journal_volume                  24
_journal_year                    1997
_chemical_formula_sum            W
_chemical_name_mineral           Tungsten
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.1926
_cell_length_b                   3.1926
_cell_length_c                   3.1926
_cell_formula_units_Z            2
_cell_volume                     32.541
_database_code_amcsd             0008080
_diffrn_ambient_temperature      2032
_exptl_crystal_density_diffrn    18.763
_cod_original_sg_symbol_H-M      'I m 3 m'
_cod_database_code               9006498
Thermal expansion of periclase (MgO) and tungsten (W) to melting temperatures Sample: T = 2171 K
Dubrovinsky, L. S.; Saxena, S. K.; Physics and Chemistry of Minerals 24 (1997) 547–550; doi:10.1007/s002690050070

data_9006499
_publ_section_title
;
 Thermal expansion of periclase (MgO) and tungsten (W)
 to melting temperatures
 Sample: T = 2171 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              547
_journal_page_last               550
_journal_paper_doi               10.1007/s002690050070
_journal_volume                  24
_journal_year                    1997
_chemical_formula_sum            W
_chemical_name_mineral           Tungsten
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.1946
_cell_length_b                   3.1946
_cell_length_c                   3.1946
_cell_formula_units_Z            2
_cell_volume                     32.602
_database_code_amcsd             0008081
_diffrn_ambient_temperature      2171
_exptl_crystal_density_diffrn    18.728
_cod_original_sg_symbol_H-M      'I m 3 m'
_cod_database_code               9006499
Thermal expansion of periclase (MgO) and tungsten (W) to melting temperatures Sample: T = 2310 K
Dubrovinsky, L. S.; Saxena, S. K.; Physics and Chemistry of Minerals 24 (1997) 547–550; doi:10.1007/s002690050070

data_9006500
_publ_section_title
;
 Thermal expansion of periclase (MgO) and tungsten (W)
 to melting temperatures
 Sample: T = 2310 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              547
_journal_page_last               550
_journal_paper_doi               10.1007/s002690050070
_journal_volume                  24
_journal_year                    1997
_chemical_formula_sum            W
_chemical_name_mineral           Tungsten
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.1979
_cell_length_b                   3.1979
_cell_length_c                   3.1979
_cell_formula_units_Z            2
_cell_volume                     32.704
_database_code_amcsd             0008082
_diffrn_ambient_temperature      2310
_exptl_crystal_density_diffrn    18.670
_cod_original_sg_symbol_H-M      'I m 3 m'
_cod_database_code               9006500
Thermal expansion of periclase (MgO) and tungsten (W) to melting temperatures Sample: T = 2450 K
Dubrovinsky, L. S.; Saxena, S. K.; Physics and Chemistry of Minerals 24 (1997) 547–550; doi:10.1007/s002690050070

data_9006501
_publ_section_title
;
 Thermal expansion of periclase (MgO) and tungsten (W)
 to melting temperatures
 Sample: T = 2450 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              547
_journal_page_last               550
_journal_paper_doi               10.1007/s002690050070
_journal_volume                  24
_journal_year                    1997
_chemical_formula_sum            W
_chemical_name_mineral           Tungsten
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.2026
_cell_length_b                   3.2026
_cell_length_c                   3.2026
_cell_formula_units_Z            2
_cell_volume                     32.848
_database_code_amcsd             0008083
_diffrn_ambient_temperature      2450
_exptl_crystal_density_diffrn    18.588
_cod_original_sg_symbol_H-M      'I m 3 m'
_cod_database_code               9006501
Thermal expansion of periclase (MgO) and tungsten (W) to melting temperatures Sample: T = 2620 K
Dubrovinsky, L. S.; Saxena, S. K.; Physics and Chemistry of Minerals 24 (1997) 547–550; doi:10.1007/s002690050070

data_9006502
_publ_section_title
;
 Thermal expansion of periclase (MgO) and tungsten (W)
 to melting temperatures
 Sample: T = 2620 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              547
_journal_page_last               550
_journal_paper_doi               10.1007/s002690050070
_journal_volume                  24
_journal_year                    1997
_chemical_formula_sum            W
_chemical_name_mineral           Tungsten
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.2079
_cell_length_b                   3.2079
_cell_length_c                   3.2079
_cell_formula_units_Z            2
_cell_volume                     33.011
_database_code_amcsd             0008084
_diffrn_ambient_temperature      2620
_exptl_crystal_density_diffrn    18.496
_cod_original_sg_symbol_H-M      'I m 3 m'
_cod_database_code               9006502
Thermal expansion of periclase (MgO) and tungsten (W) to melting temperatures Sample: T = 2720 K
Dubrovinsky, L. S.; Saxena, S. K.; Physics and Chemistry of Minerals 24 (1997) 547–550; doi:10.1007/s002690050070

data_9006503
_publ_section_title
;
 Thermal expansion of periclase (MgO) and tungsten (W)
 to melting temperatures
 Sample: T = 2720 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              547
_journal_page_last               550
_journal_paper_doi               10.1007/s002690050070
_journal_volume                  24
_journal_year                    1997
_chemical_formula_sum            W
_chemical_name_mineral           Tungsten
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.2094
_cell_length_b                   3.2094
_cell_length_c                   3.2094
_cell_formula_units_Z            2
_cell_volume                     33.058
_database_code_amcsd             0008085
_diffrn_ambient_temperature      2720
_exptl_crystal_density_diffrn    18.470
_cod_original_sg_symbol_H-M      'I m 3 m'
_cod_database_code               9006503
Thermal expansion of periclase (MgO) and tungsten (W) to melting temperatures Sample: T = 2774 K
Dubrovinsky, L. S.; Saxena, S. K.; Physics and Chemistry of Minerals 24 (1997) 547–550; doi:10.1007/s002690050070

data_9006504
_publ_section_title
;
 Thermal expansion of periclase (MgO) and tungsten (W)
 to melting temperatures
 Sample: T = 2774 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              547
_journal_page_last               550
_journal_paper_doi               10.1007/s002690050070
_journal_volume                  24
_journal_year                    1997
_chemical_formula_sum            W
_chemical_name_mineral           Tungsten
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.2116
_cell_length_b                   3.2116
_cell_length_c                   3.2116
_cell_formula_units_Z            2
_cell_volume                     33.126
_database_code_amcsd             0008086
_diffrn_ambient_temperature      2774
_exptl_crystal_density_diffrn    18.432
_cod_original_sg_symbol_H-M      'I m 3 m'
_cod_database_code               9006504